http://www.sciencepublishinggroup.com/j/css doi: 10.11648/j.css.20170204.13
Tribological Properties of Multilayer TiN and MoS
, Sorin Cioc1
, Carmen Cioc2
, Ahalaptiya H. Jayatissa1
Nanotechnology and MEMS Laboratory, Department of Mechanical, Industrial, and Manufacturing Engineering (MIME), The University of Toledo, Toledo, USA
Department of Engineering Technology, The University of Toledo, Toledo, USA
firstname.lastname@example.org (A. H. Jayatissa)
To cite this article:
Omer Ahmed, Sorin Cioc, Ahalaptiya H. Jayatissa. Tribological Properties of Multilayer TiN and MoS2 Thin Films. Colloid and Surface Science. Vol. 2, No. 4, 2017, pp. 137-142. doi: 10.11648/j.css.20170204.13
Received: May 22, 2017; Accepted: May 25, 2017; Published: October 13, 2017
Abstract:This paper presents tribological behavior of titanium nitride and molybdenum sulfide thin film coatings on a workpiece. The titanium nitride films were coated by RF magnetron sputtering method and molybdenum sulfide films were coated by vacuum thermal evaporation. Titanium nitride is a hard ceramic materials, which has excellent mechanical properties. However, the friction coefficient of titanium nitride is rather high. To improve the tribological properties of the titanium nitride films, a thin layer of molybdenum sulfide was coated as a solid lubricant. The results showed a substantial decrease in the coefficient of friction of dual-layered MoS2 over TiN compared with the titanium nitride film or as-received aluminum substrate. The low coefficient of friction can directly be correlated to the MoS2 layer whereas the TiN film acts as a robust and durable base material. The coefficient of friction was measured using a pin on a disc tribometer with a steel pin as the counter face. Our results demonstrated that the coating of MoS2 over TiN has a low coefficient of friction. In addition, it was also found that wear resistance of MoS2 coated TiN was better than both MoS2 and TiN films.
Keywords:Coefficient of Friction, Titanium Nitride, Molybdenum Sulfide, Tribology
Coatings are often used in manufacturing to improve mechanical, tribological, and aesthetic properties of workpieces. These coatings have several applications that range from lubrication to formation of hard protective layers. Different kinds of coatings are available depending on the applications. Hard ceramic coatings are used for coating of machine tools and protect underneath material, whereas soft lubricating coatings are employed to improve the lubricity in places where fluid lubricants cannot be used. Mechanical and tribological properties of thin films can be improved by application of multilayer coatings. Multilayer coatings have resulted in enhanced properties such as decreased coefficient of friction, increase in load bearing capacities, and wear life (durability) for different materials [1-9]. Several type of coatings such as composite, hybrid, multiphase, or gradient films have been developed for improving the tribological properties by combination of materials [1, 3, 4]. The combinations of these layers also depend on the cost and
throughput of manufacturing. Based on quality, the film surfaces can be classified into either anti-friction coatings determined by low friction or anti-wear coatings characterized by high hardness .
Titanium nitride (TiN) is a widely used ceramic coating due to its excellent mechanical properties and high resistance to wear and corrosion . TiN is coated as thin films to improve the mechanical performance of substrates [1, 11]. Although TiN has good durability, it has a high coefficient of friction (> 0.62). It is vital to improve the frictional properties of TiN as it is mostly used in machine tools and materials having contact . Molybdenum sulfide (MoS2) is a commonly used dry solid lubricant, which has a low coefficient of friction in the range of 0.09 - 0.15 as a single layered film on the working surfaces. MoS2 have also been used as a composite/additive to lower friction in composite or multilayer coatings [3, 14, 16]. An optimum balance of good durability and low coefficient of friction can be obtained by combining the properties of TiN and MoS2 films.
20]. coating of TiN + MoS composite were carried out by closed-field magnetron sputtering method and the thickness of 2 µm showed the average coefficient of friction around 0.35 . The composition of MoS2 in surface coatings showed decrease in friction coefficient from 0.3 to 0.05, but the results were irregular due to its low hardness . MoS2 coatings provided a very low coefficient of friction with an average value around 0.08 in different working environments .
In this study, MoS2 were deposited on pre-fabricated TiN films. The TiN and MoS2 films were coated separately in different processes & environments to distinguish between the layers. TiN films were coated using RF magnetron sputtering and MoS2 films were coated using vacuum thermal evaporation technique. The friction measurements were made using a pin-on-disc tribometer with a steel counter face pin and the substrate rotating at a constant speed. The effect of wear and durability were studied by changing the applied normal loads.
2. Experimental Procedure
The TiN and MoS2 films were deposited on the as-received Al substrates. The Al grade used was alloy 1100 as it is commonly used in general fabrication and metal spinning. The aluminum alloy 1100 had composition of 99.88% Al, 0.1% Copper and 0.02% residuals . Prior to deposition, the substrates were cut into appropriate dimensions (8 cm x 8cm, thickness 0.8 mm) and cleaned with soap and water for removing grease and dirt. The substrates were then sonicated in a mixture of acetone, isopropanol alcohol and distilled water for removing surface contaminations. All components were analytical grade and were used as received. The thin films were coated on these Al substrates by physical vapor deposition techniques.
The TiN thin films were deposited by reactive radio frequency (RF) magnetron sputtering method on Al substrates. The deposition was carried out a pressure inside the chamber was maintained at 1x10-6 Torr with the help of a multi-stage vacuum pump throughout the deposition time. After the required pressure was obtained, the vacuum chamber was purged with argon to remove any oxygen in the chamber. Then a mixture of Ar and N2 gases (1: 1) were introduced and pressure was adjusted to 30 mTorr. Titanium nitride was deposited for 120 min using RF power of 250 W. The average thickness of the film obtained was in the range of 325±10 nm.
Vacuum thermal evaporation technique used for the deposition of molybdenum sulfide (MoS2) films. This process provided a higher deposition rates and was suitable for depositing MoS2. In this technique, the MoS2 powder to be deposited was evaporated/sublimated at a temperature higher than 1185°C. The TiN coated Al substrates were coated at a pressure of 10-6 Torr using a Mo crucible filament. MoS2 powder of 99.9% purity with average particle size of 44 microns was used as the source material. The average the thickness of MoS2 films were around 350 nm.
The tribology tests were conducted on a custom-built pin-on-disc tribometer (figure 1). It measures the frictional force exerted on the surface of the substrate by deflection of the stationary pin. The coated substrates were mounted on a steel holder attached to the motor. The counter face steel pin was placed on the surface of the disc so that it touches the substrate surface. The pin was rigidly attached to strain gauges. A normal force was exerted on the pin due to its own weight and external application of applied normal force. Additional weights were used to increase applied normal force for different experiments. The applied normal load was increased by the use of static weights such that the force acts tangentially to the substrate surface. The deflection was measured with the set of strain gauges that are interfaced to a computer running LabVIEWTM. Real-time deflection and frictional force data were collected via a data acquisition system and custom LabViewTM software. The surface roughness of the pin was 110 nanometers. A constant speed of 150 rpm was maintained and loads of magnitude, 0.25 N, 0.375 N, and 1.1 N were used. All the readings were recorded at room temperature and ambient air-conditions (1 atm). The forces acting on the substrate during the test are illustrated in figure 1.
Figure 1. Schematic of pin on disc tribometer.
3. Results and Discussion
3.1. Coefficient of Friction
coefficient of friction of 0.14, which is comparable with the sputter deposited MoS2 films, which have the average frictional value of 0.12 [12, 19].
Table 1. Average coefficient of friction of coatings at different loads.
Layer Contact pressure
180 MPa 270 MPa 800 MPa
MoS2/Al 0.1 0.14 0.14
MoS2/TiN/Al 0.09 0.14 0.15
The comprehensive effect of friction coefficient MoS2 over TiN coating and TiN coating is shown in figure 2. The friction coefficient of the coated substrates is plotted versus number of cycles in figure 2 and figure 3. The coefficient of friction of MoS2 over TiN coating was significantly lower than the TiN coating as presented in figure 2. During the period of 20,000 cycles, the coefficient of friction of MoS2 over TiN behaved consistently and displayed a low value. These measurements were recorded at applied normal load of 0.375 N on the counter face steel pin. TiN provided a good protection for the base Al but it did not demonstrate good frictional properties. The frictional coefficient of TiN remained in the range of 0.59 to 0.77. Also, the coefficient of friction of MoS2 over TiN was in a lower range of 0.12 to 0.15 for identical speed and normal load. The MoS2 coatings studied in several other studies exhibited similar results with low coefficient of friction of approximately 0.1 [12, 15, 16-20]. A MoS2 film deposited by sputtering technique with film thickness of one micron showed steady state coefficient of friction of 0.08 at ambient conditions . J. Haider et al  reported that the MoS2 deposited by magnetron sputtering resulted in film with average coefficient of friction of 0.15. The addition of MoS2 on the substrate improved coefficient of friction. The decreased coefficient of friction shows that the MoS2 layer provides better lubricity in steady state conditions. Lower friction coefficients were obtained by the incorporation of MoS2 within a hard matrix such as TiN by co-deposition, which also resulted in drop in hardness . In this case, the coefficient of friction was inversely proportional to hardness of the coatings.
Figure 2. Coefficient of friction of TiN and MoS2 over TiN thin films.
Single layered MoS2 and dual layered MoS2 over TiN provided similar coefficient of friction as shown in figure 3.
The difference in friction coefficient is low with an average of 0.14. Reduced values of coefficient of frictions were obtained (in figure 3) as the top most layer comprised of MoS2 films. The top layer of both the substrates contained similar MoS2 films and materials and they were deposited using identical techniques and parameters. Another study indicated that the TiN + MoS2 composite coating exhibited an average steady state coefficient of friction of 0.32 with drastic changes throughout the testing period . The films of TiN+MoS deposited by magnetron sputtering also showed a higher coefficient of friction of 0.35 . These results suggest that the homogeneous MoS2 layer proved to be suitable solid lubricant layer for reducing coefficient of friction.
Figure 3. TiN-MoS2 coatings vs MoS2 coatings (a) Normal load = 0.375 N
(b) Normal load = 1.1 N.
friction. The increased coefficient of friction value of MoS2 film is closer to coefficient of friction of standard Al alloy 1100, which was used as the substrate material. The dual layered MoS2 over TiN coating showed a better durability than single layered MoS2. In the MoS2 over TiN film coatings, the MoS2 layer wore out after 300 s, but it still provided lubricity and displayed decreased coefficient of friction for MoS2 over TiN film substrates.
Figure 4. Wear and durability, MoS2, MoS2-TiN & Wet TiN.
The MoS2 layer had positive effect over the coefficient of friction of the substrates after deteriorating. The MoS2 debris was presented at surface interaction between pin and substrate surface. The suspended MoS2 fragments acted as partial dry solid lubricant in this case. The average steady state coefficient of friction of plain TiN coatings was 0.62; but the average coefficient of friction of TiN layer after wearing of MoS2 layer was found to be 0.21. This decrease in coefficient of friction indicated the effect of MoS2 particles on the lubricity of the substrate after the MoS2 film was scratched. The MoS2 debris particles provided lubrication effect in the case of single layered MoS2 film coating, as there was a considerable decrease in coefficient of friction in Al. The average coefficient of friction of as received Al 1100 was 0.7. However, the coefficient of friction of Al 1100 after the MoS2 film was scratched was found to be 0.6. These results suggested that the interface of MoS2/TiN has some significant effect on tribology performance. Authors plan to investigate these phenomena in the future.
Figure 5. Relationship between applied normal load and contact pressure.
Figure 6. Surface morphology for different loads (a) MoS2 film (b) MoS2
over TiN films.
The effect of lubrication of MoS2 is apparent in figure 6. The lubrication effect of water on plain TiN coatings is compared to lubricity provided by MoS2 layer. Water acted as an effective lubricant and provided lower COF average of 0.34 compared to 0.62 of dry TiN coatings. The effect of wear was also decreased with consistent performance throughout the testing period.
3.2. Surface Interactions
The actual load acting on the substrate surface through the pin changes with different loads and this changes coefficient of friction and area of contact. This phenomenon can be explained using Hertzian contact theory and by calculating Hertzian contact pressure for the applied normal loads and geometry of the setup. Hertzian contact pressure can be calculated by using the following set of formulae ,
where, a is contact radius, E is Young's Modulus, P is applied normal load, R- radius of the pin and ν- poisson’s ratio. Maximum Hertzian contact (Pmax) pressure is given by
1 = − pin + − plate
E E E
The relationship between the applied normal load and the maximum Hertzian contact pressure is linear as calculated from eq. (2). The results show a linear relationship of applied normal load and maximum Hertzian contact pressure. As the applied normal load increases the maximum Hertzian contact pressure also increases with corresponding magnitude. The change in contact pressure had direct influence on frictional coefficients and wear behavior for MoS2 and MoS2 over TiN film coatings. The maximum Hertzian contact pressures for 0.25, 0.375 and 1.1 N were found to be 263, 300 and 430 MPa, respectively.
diameter that was measured by optical microscope. The empirically calculated contact area and contact pressure acting on the surface are displayed in figure 5. The contact area of the steel pin is 0.00138 mm2. The contact pressures for 0.25, 0.375 and 1.1 N were found to be 180, 270 and 800 MPa, respectively.
Figure 6 shows the surface images of MoS2 and MoS2 over TiN after application of different loadings in tastings. The difference in width of wear tracks in figure 6 was explained by increase in contact pressure. The wear for 15,000 cycles in the dual layered MoS2 over TiN coating was similar to the single layered MoS2 coating as shown in figure 6.
Figure 7. Wear tracks for (a)MoS2 and (b)MoS2 over TiN films.
Figure 7 shows the effect of wear between MoS2 and MoS2 over TiN films for long-term applications. The difference in wear tracks is between the two coatings subjected to identical load, speed, and other conditions. In the case of MoS2 film, the wear was apparent and the wear track was rough exposing the bare substrate material (Al). Due to wear and tear, the width of the track was irregular on MoS2 coated substrate. This resulted in formation of a rugged wear track with high coefficient of friction after wear. Whereas, in MoS2 over TiN film, the TiN below the MoS2 layer prevented the substrate from excessive damage and wear. The wear track also had uniform width and substrate material was not scarred.
The MoS2 over TiN dual layered coatings proved to be a good option for increasing the lubricity of the TiN coatings that are often used in machine tools as hard ceramic coatings.
The MoS2 over TiN dual layered coatings have advantages over the TiN+MoS composite coatings. The dual layered MoS2 over TiN films obtained in this study have lower coefficient of friction of 0.15 compared with the TiN+MoS composite coatings that have a higher coefficient of friction of 0.35 .
MoS2 has been used as a solid lubricant because it has a lamellar structure, which the layers can slide along each other. It is known that MoS2 doesn’t function very well in a wet environment and causes corrosion of metal surfaces due to galvanic corrosion between Molybdenum disulfide and metals. In this study, however; reduced friction coefficient after addition of water into the MoS2 surface after coating on TiN. Furthermore, TiN is an anticorrosion materials and thus, it durability of MoS2 in wet environment might be enhanced by coating dual layer of MoS2 and TiN.
The coatings of MoS2 films, TiN layers and MoS2 on TiN were carried out by RF magnetron sputtering and vacuum thermal evaporation. These films were investigated for their tribological properties in sliding contact (pin-on disc tribometer) in ambient conditions by varying the applied normal load. Although the coating of TiN provided hard protective layers for the base materials, its coefficient of friction is as high as 0.6. A thin film of MoS2 was proven a reliable and dry solid lubricant with the coefficient of friction as low as 0.14. By combining the properties of these two materials, a dual layered coating with contact layer being MoS2 was fabricated to utilize the coefficient of friction of MoS2 and anti-wear properties of TiN. The experimental results exhibited that the proposed novel dual layered coatings were successful with the average coefficient of friction of dual layer remained close to that of MoS2. Study suggested that the coating of MoS2 over TiN was a useful self-lubricating coating for long-term applications. Thin films of MoS2 can be deposited on TiN coated substrates and machine tools. MoS2 over TiN dual layered coatings can also be applied in places where conventional lubrication techniques are difficult to use effectively such as in high temperature environments, space vehicles, food industry equipment, and bearings.
 X. T. Zenga, S. Zhangb, C. Q. Sunc, Y. C. Liua, Nanometric-layered CrN/TiN thin films: mechanical strength and thermal stability, Thin Solid Films, 424 (2003) 99–102
 J. Li, X. Zeng, T. Ren and E. Heide, The Preparation of Graphene Oxide and Its Derivatives and Their Application in Bio-Tribological Systems, Lubricants 2 (2014)137-161.
 S. K. Field, M. Jarratt, D. G. Teer, Tribological properties of graphite-like and diamond-like carbon coatings, Tribology International, 37 (2004) 949–956.
 Abadias, G., Michel, A., Tromas, C., Jaouen, C., Dub, S. N.: Stress, interfacial effects and mechanical properties of nanoscale multilayered coatings. Surface & Coatings technology 202, 844-853 (2007).
 G. Ma, L. Wang, H. Gao, J. Zhang, and T. Reddyhoff, The friction coefficient evolution of a TiN coated contact during sliding wear, Applied Surface Science, 345 (2015) 109–115.
 J. L. Mo and M. H. Zhu, Tribological oxidation behaviour of PVD hard coatings. Tribology International 42(2009)1758-1764.
 M. Gubischa, Y. Liub, L. Spiessa, H. Romanusa, S. Krischokb, G. Eckec, J. A. Schaeferb, Ch. Knedlika, Nanoscale multilayer WC/C coatings developed for nanopositioning: Part I. Microstructures and mechanical properties, Thin Solid Films, 488 (2005) 132–139
 Rivera-Tello, C. D., Broitman, E., Flores-Ruiz, F. J., Jimenez, O., Flores, M.: Mechanical properties and tribological behavior at micro and macro-scale of WC/WCN/W hierarchical multilayer coatings. Tribology International 101, 194-203 (2016).
 Sangiovanni, D. G.: Transition metal nitrides: Alloy design and surface transport properties using Ab-initio and classical computational methods. Linkoping Studies in Science and Technology, dissertation no. 1513 (2013).
 Kelly, P. J., Braucke, T., Liu, Z., Arnell, R. D., Doyle, E. D.: Pulsed DC titanium nitride coatings for improved tribological performance and tool life. Surface & Coatings Technology 202, 774-780 (2007).
 Haider, J., Rahman, M., Corcoran, B., Hashmi, M. S. J.: Deposition and characterization of hard- solid lubricant coating by closed field magnetron sputtering. Surface & Coatings Technology 200, 1080-1083 (2005).
 Shriver, D. F., Atkins, P. W., Overton, T. L., Rourke, J. P., Weller, M. T., Armstrong, F. A.: Inorganic Chemistry. New York: W. H. Freeman (2006).
 Gangopadhyay, S., Acharya, R., Chattopadhyay, A. K., Paul, S.: Effect of substrate bias voltage on structural and mechanical properties of pulsed DC magnetron sputtered TiN-MoSx composite coatings. Vacuum 84, 843-850 (2010).
 Rahman, M., Haider. J., Dowling, D. P., Duggan, P., Hashmi, M. S. J.: Deposition of magnetron sputtered TiN + MoSx coating with Ti-TiN graded interlayer. Surface & Coatings Technology 200, 1071-1075 (2005).
 Jing, Y., Luo, J., Pang, S.: Effect of Ti or TiN co deposition on the performance of MoS2-based composite coatings. Thin Solid Films 461, 288–293 (2004).
 Bhaduri, D., Kumar, R., Jain, A. K., Chattopadhyay, A. K.: On tribological behavior and application of TiN and MoS2-Ti composite coating for enhancing performance of monolayer cBN grinding wheel. Wear 268, 1053-1065 (2010).
 Xu, G., Zhou, Z., Liu, J., Ma, X.: An investigation of fretting behavior of ion-plated TiN, magnetron sputtered MoS2 and their composite coatings. Wear 225-229, 46-52 (1999).
 C. G. Dunckle, M. Aggleton, J. Glassman, P. Taborek, Friction of molybdenum sulfide–titanium films under cryogenic vacuum conditions, Tribology International 44 (2011) 1819– 1826
 Goller, R., Torri, P., Baker, M. A., Gilmore, R., Gissler W.: The deposition of low friction TiN-MoSx hard coatings by a combined arc evaporation and magnetron sputter process. Surface coatings and technology 120-121, 453-457 (1999).
 Budynas, R., Nisbett, K.: Shigley’s mechanical engineering design. McGraw-Hill series in mechanical engineering, 10th edition, 3.19 (2014).